OPEN

Received: 14 October 2016 Accepted: 22 May 2017 Published: xx xx xxxx

Dielectric properties of complex magnetic field induced states in PbCuSO4(OH)2 T. Mack, A. Ruff, H.-A. Krug von Nidda, A. Loidl & S. Krohns Spin spirals, which coexist with collinear spin order in linarite PbCuSO4(OH)2, indicate electrical polarisation textures of spin-multipolar phases. We derive experimental evidence by a detailed investigation of the magnetic-field dependent dielectric and electric polarization properties at low temperatures. Linarite exhibits a quasi-one-dimensional frustrated S = ½ spin chain, which forms 3D spin-spiral order in zero magnetic field for T ¼5. But, tuning the α parameter, instabilities of spiral states like their vector chirality can result in various spin multipolar phases (SMP), as quadrupolar bond-nematic state (p = 2)6 or multi magnon-bound states (p > 2)1. The p-values denote finite elementary magnetization steps as a function of magnetization and frustration7. For the low magnetization regime, in the ordered state (T 2, which may compete with exotic longitudinal collinear spin-density waves (SDWp), was given by Willenberg et al.1. Even multi-magnon bound states reaching p = 9 are achieved by tuning the frustration parameter in the vicinity of the magnetic saturation field. Above magnetic saturation in fields of ms > 6 T, field induced spin-polarized states evolve. Here, the critical fields depend on the crystallographic directions where the magnetic field is applied. Interestingly, the saturation fields are by a factor of 5 smaller than for LiCuVO422. This allows to investigate these complex magnetic phases in fields up to 10 T. In this paper, we study in detail the electrical polarization properties of linarite as function of magnetic field and temperature. For LiCuVO413, which is a prototypical example to test for switching of electrical polarization via a magnetic field, the polarization P is evolved only, if the vector product of spin spiral axis e and propagation of the spin spiral Q is finite, i.e. P ∝ e × Q8. In contrast, linarite was ascribed to show no rotation of the spiral axis e under an applied magnetic field due to its monoclinic structure1. However, we provide a thorough dielectric characterization as function of magnetic fields applied in a, b and a⊥-direction and reveal the correlation of magnetic and electrical order. In the present experiment only a and b directions are well defined with respect to the external fields. Due to fact, that the crystal structure is monoclinic, the c direction of this sample is not well known. At TN a clear dielectric anomaly indicates the FE transition. This confirms the multiferroic nature of linarite16. Further significant dielectric signatures are found depending on crystallographic direction, applied magnetic fields and temperature. These transitions are discussed in terms of remnant switchable spin spirals and electrical polarization texture of SMPs. We prove the sample quality of a natural grown single crystal from a mine in Lavrion (Greece) performing temperature dependent magnetic susceptibility χ (Fig. 1a) and specific heat measurements cp (Fig. 1b). The magnetic susceptibility χ was analysed along a, b and a⊥ crystallographic directions in an applied magnetic field of H = 0.1 T. A distinct peak anomaly shows up around 5 K for all directions, followed by a step-like decrease at T = 2.85 K (inset of Fig. 1a). The latter denotes the antiferromagnetic ordering and is in good agreement with previously published results from linarite crystals of different origins1, 15, 27. The lines represent a reasonable fit of χ using a numerical approximation of an isotropic linear one-dimensional antiferromagnetic spin ½ chain28, 29. From these fits we determine an average antiferromagnetic exchange coupling of J/kB = 3,7 K. The high temperature Curie-Weiss behaviour signals a Curie-Weiss temperature close to 0 K indicating competing nearest and next nearest neighbour exchange. The inset of Fig. 1a indicates slightly anisotropic g-values with maximum value for H || a in fair agreement with literature16, 30. Figure 1b show specific heat measurements along a direction for various applied magnetic fields. The peak anomaly in cp at TN and its magnetic field dependence originating from long-range spin spiral formation confirm the literature1, 15, 27. Both measurements evidence reasonable sample quality, which allow the investigation of electrical polarization of the complex magnetic phases close to TN.

Spiral spin configuration

In analogy to LiCuVO413, Fig. 2 schematically shows the ground state of the spiral spin configuration as function of magnetic field. For clarity reasons only the magnetic CuO4 plaquetts in ribbon structure are depicted. The spin configuration of the ground state has been systematically characterized by neutron diffraction26, magnetization22, 27, NMR1 and specific heat measurements27. The spin spiral exhibits a modulation vector Q parallel to the b direction and lies in a plane spanned by b and a vector tilted by 27° from a. Thus, the spin spiral axis e is almost parallel to crystallographic [−1 0 1] direction. In this case inverse Dzyaloshinskii-Moryia interactions (DMI) or spin currents induce an electric polarization in e⊥, i.e., parallel to [1 0 1] direction. In contrast to ref. 1, we assume a rotation of the spin-spiral axis e at a critical field H1 into the applied external magnetic field direction, while the modulation vector is unchanged. Between H1 and H2, namely for H || a⊥ the polarisation is along a and for H || Scientific Reports | 7: 4460 | DOI:10.1038/s41598-017-04752-z

2

www.nature.com/scientificreports/

Figure 2. Schematic sketch of the spin configurations in the magnetically ordered phases of PbCuSO4(OH)2 as function of external magnetic field. The switching of the spin spiral for the different magnetic field directions is indicated in analogy to LiCuVO4. In the ground state the elliptical helix shows a component in b-direction while the other component is forming an angle of 27° with the a-axis (spiral axis e almost [−1 0 1]). H1 and H2 indicate phase boundaries between the different magnetic phases.

a along the a⊥ direction. Here, we use a⊥, which is perpendicular to a, that means a direction counter clockwise tilted by 13° from c towards a. In case of H || b above H1, the spiral axis is along the modulation vector, which prevents polarisation via P ∝ e × Q. However, in the vicinity of H1 instabilities of the spin spirals result in SMPs1. A fully spin-polarized state evolves with a collinear spin structure for H > H2. For linarite the upper critical field H2 depends on the crystallographic direction and is of the order of 6 to 8 T.

Magnetic field along a⊥-direction

As indicated in Fig. 2 three cases above H1 are of interest: i) H || a⊥ in Fig. 3, ii) H || b in Fig. 4 and iii) H || a shown in Fig. 5, respectively. In Fig. 3a we present the temperature and magnetic field dependent deviations of the dielectric constant in parts per thousand (‰). This was calculated using the static dielectric constant in zero magnetic field at T = 3.5 K. The external magnetic field up to 7 T was applied along the a⊥-direction and the dielectric properties as well as the polarization measured in a-direction. Significant peak anomalies in Δε’ emerge for H H1 Δε’(T) follows rather the phase boundary of the blue-dashed area, which denotes the SMP, than the one of the spin spirals (grey area). The SMP boundary has been identified from NMR studies1 and specific heat measurements27. The latter ones are depicted in Fig. 4c as orange triangles and confirm the phase boundaries (c.f. phases I, II, IV and V of refs 1 and 27) revealed by dielectric, pyrocurrent and magnetocurrent measurements. The results of dielectric spectroscopy as an indirect measure of the spin spirals indicate a polar texture of a SMP, where close to the saturation field instabilities of spin spirals persist. In Scientific Reports | 7: 4460 | DOI:10.1038/s41598-017-04752-z

3

www.nature.com/scientificreports/

Figure 3. Dielectric properties at 300 Hz with E || a of a PbCuSO4(OH)2 single crystal with magnetic field along the a⊥ direction. (a) Temperature dependent dielectric constant for various magnetic fields. The dielectric constant is normalized to a constant value and deviations are shown in parts per thousand (‰). The inset illustrates the spin configuration between H1 and H2. (b) Temperature dependent electrical polarization performed for different magnetic fields, with a poling field Epol = 2 kV/cm. (c) (T,H) phase diagram constructed using results from the present work; the grey shaded area indicates the rotated spin spiral state. The inset shows magnetic field dependent dielectric constants and polarization at 1.7 and 1.9 K, respectively (lines are drawn to guide the eye). Fig. 4b the onset of polarisation and the polar strength are shown, which are even for H H1 is sensitive to a polar order resulting from instabilities of various spin spirals within the SMP. This further indicates that the observed polarization is a function of magnetic and thermal treatment and only detectable by dielectric measurements, when starting in the paramagnetic disordered state above TN. The anomalies of Δε’(T) for H > 2 T are then related to the polar moment of a locally persisting spin spiral as a consequence of fluctuations within the frustrated spin chain system.

Magnetic field along a-direction

Figure 5 shows the results of dielectric and polarization measurements for E || a⊥ and H || a. For this case we expect a flip of the spin spiral axis from e || [−1 0 1] into crystallographic a direction at H1 ≈ 3.5 T. As shown in Fig. 2, this represents the “switching” case of the polarization P, which is aligned along [1 0 1] for H